|Year : 2018 | Volume
| Issue : 2 | Page : 136-141
|The impact of artificially caries-affected dentin on bond strength of multi-mode adhesives
Andressa Cargnelutti Follak1, Leonardo Lamberti Miotti1, Tathiane Larissa Lenzi2, Rachel de Oliveira Rocha2, Fabio Zovico Maxnuck Soares3
1 School of Dentistry, Federal University of Santa Maria, Santa Maria, Brazil
2 Stomatology, Federal University of Santa Maria, Santa Maria, Brazil
3 Restorative Dentistry, Federal University of Santa Maria, Santa Maria, Brazil
Click here for correspondence address and email
|Date of Submission||20-Nov-2017|
|Date of Decision||19-Dec-2017|
|Date of Acceptance||05-Feb-2018|
|Date of Web Publication||22-Mar-2018|
| Abstract|| |
Aim: The aim of this study is to evaluate the impact of dentin condition on bond strength of multi-mode adhesive systems (MMAS) to sound and artificially induced caries-affected dentin (CAD).
Methods: Flat dentin surfaces of 112 bovine incisors were assigned to 16 subgroups (n = 7) according to the substrate condition (sound and CAD– pH-cycling for 14 days); adhesive systems (Scotchbond Universal, All-Bond Universal, Prime and Bond Elect, Adper Single Bond Plus and Clearfil SE Bond) and etching strategy (etch-and-rinse and self-etch). All systems were applied according to the manufacturer's instructions, and resin composite restorations were built. After 24 h of water storage, specimens were sectioned (0.8 mm2) and submitted to the microtensile test.
Statistical Analysis: Data (MPa) were analyzed using three-way analysis of variance and Tukey's test (α = 0.05).
Results: MMAS presented similar bond strength values, regardless etching strategy in each substrate condition. Bond strength values were lower when MMAS were applied to CAD in the etch-and-rinse strategy.
Conclusion: The etching strategy did not influence the bond strength of MMAS to sound or CAD, considering each substrate separately. However, CAD impact negatively on bond strength of MMAS in etch-and rinse mode.
Keywords: Bond strength; caries-affected dentin; micro-tensile; multi-mode adhesive
|How to cite this article:|
Follak AC, Miotti LL, Lenzi TL, Rocha Rd, Maxnuck Soares FZ. The impact of artificially caries-affected dentin on bond strength of multi-mode adhesives. J Conserv Dent 2018;21:136-41
|How to cite this URL:|
Follak AC, Miotti LL, Lenzi TL, Rocha Rd, Maxnuck Soares FZ. The impact of artificially caries-affected dentin on bond strength of multi-mode adhesives. J Conserv Dent [serial online] 2018 [cited 2018 Jul 18];21:136-41. Available from: http://www.jcd.org.in/text.asp?2018/21/2/136/228263
| Introduction|| |
Following the trend to obtain straightforward materials and techniques universal or multi-mode adhesives systems were developed to be used both in etch-and-rinse or self-etch approaches. This versatility allows the professional decide the most appropriate protocol for each clinical situation. The multi-mode adhesive systems (MMAS) have been assessed in the past years,,,,,, and it has been reported that their in vitro performance is dependent on the adhesive strategy, especially regarding enamel bonding. However, for dentin, there is no consensus on the literature about the influence of etching strategy and the long-term performance of multi-mode adhesives. Besides that, caries-affected dentin (CAD), a clinically relevant substrate  has not been considered in in vitro evaluations of MMAS. Considering that, the differences in composition and microstructure of CAD compared to sound one and the consequently lower bond strength values found to this substrate in studies with previous adhesive systems ,, it seems reasonable to include CAD on MMAS' evaluations.
A recent study  showed that the immediate bond strength of a universal adhesive system was not influenced by the etching approach either by the dentin condition (artificially caries-affected primary or permanent dentin). However, this study assessed only one multi-mode adhesive system, and a gap remains about the performance of universal adhesives on clinically relevant substrates as CAD.
Therefore, the aim of this in vitro study was to evaluate the influence of dentin condition– sound or artificially-induced caries-affected on bond strength performance of three MMAS, using two etching strategies. The null hypotheses tested were as follows: (1) different MMAS present similar bond strength irrespective of the etching mode, and (2) the bond strength of MMAS is not influenced by dentin condition.
| Methods|| |
One hundred and twelve freshly extracted bovine incisors were used in this study. They were selected and stored previously in chloramine at 4°C for a maximum of 30 days.
The root was removed using a diamond disc in a high-speed handpiece. The buccal surfaces were ground under water-cooling using a 100-grit SiC paper in a grinder-polisher machine (EcoMet 250, Buehler; Illinois, USA) obtaining flat dentin surfaces, then manually polished using 600-grit SiC paper under water for the 60s rendering a standardized smear layer.
Artificial caries induction– artificially caries-affected dentin
The teeth were randomly assigned into two groups according to the substrate (sound and artificially CAD). Teeth allocated to sound dentin were immersed in distilled water only, and those of CAD group were exposed to artificial caries induction with a pH-cycling model., They were individually submitted to immersion for 8 h in 10 ml of demineralizing solution (2.2 mM CaCl2, 2.2 mM NaH2PO4, 50 mM acetic acid, adjusted pH of 4.8 with 1M KOH) and for 16 h in the same volume of remineralizing solution (1.5 mM CaCl2, 0.9 mM NaH2PO4, 0.15 mM KCl with adjusted pH of 7.0). Solutions' pH was confirmed and replaced every cycle for 14 days and at each interval, specimens were washed with deionized water and dried with paper towels.
Bonding and restorative procedures
Teeth from each substrate (sound dentin and CAD) were randomly reallocated (RANDOM. ORG, Randomness and Integrity Services Ltd.; Dublin, Ireland) to 8 subgroups according to the adhesive system and etching strategy (n = 7). Three multi-mode adhesives were evaluated as follows: Scotchbond Universal (SU), all-bond universal (AB) and Prime and Bond Elect (PB). All materials were applied in either self-etch (SE) or etch-and-rinse (ER) protocols. As control groups for each strategy, a two-step etch-and-rinse Adper Single Bond Plus (SB) and a two-step self-etch Clearfil SE Bond (CS) were used. All adhesive systems were applied strictly according to the manufacturer's instructions [Table 1].
|Table 1: Adhesive systems (manufacturers and batch number), composition and application mode*|
Click here to view
After hybridization, a composite block (10 mm × 7 mm × 6 mm) (Filtek Z250, EA2, 3M ESPE; St. Paul, MN, USA) was build up in three increments individually light cured for 20 s using a led curing unit (Emitter B, Schuster; Santa Maria, RS, Brazil), with an output of 600 mW/cm 2, monitored with a radiometer. All specimens were stored in distilled water at 37°C for 24 h.
Microtensile bond strength (the microtensile bond strength)
Specimens were sectioned in two axes under water-cooled diamond saw in a cutting machine (Labcut 1010, Extec Co; Enfield, CT, USA) by a single blinded operator, obtaining stick shaped specimens (approximately 0.8 mm 2) measured individually with a digital caliper (Carbografite; Petrópolis, RJ, Brazil).
Specimens were fixed to metallic devices (Odeme Medical and Dental; Joaçaba, SC, Brazil) with cyanoacrylate glue (Three Bond Super Gel, ThreeBond Ind. E Com. Ltda.; Diadema, SP, Brazil) and submitted by a single and blinded operator to microtensile test in a universal testing machine (EMIC; Sao José dos Pinhais, PR, Brazil) at a crosshead speed of 1 mm/min until fracture. Specimens that failed before the test, were recorded as pretesting failures (PTF). For PTF, a mean between zero and the lower bond strength obtained was calculated, and hence, a value of 4 MPa was attributed and included in the bond strength means. All fractured specimens were observed under ×40 stereoscope (Discovery. v20, Zeiss; Gottingen, Germany) to identify and classify the type of failure as adhesive/mixed or cohesive (dentin or resin).
For the analysis, the tooth was the experimental unit, and hence, the mean values of all specimens from each tooth were calculated, and the average value of the 7 teeth was calculated. The sample size was previously estimated considering a coefficient of variation of 20% and a power of 80%. Three factors were considered for analysis: adhesive system (AB, PB, SU, SB, and CS), bond strategy (ER and SE), and dentin condition. Normality of data was confirmed using Kolmogorov–Smirnov test. Three-way analysis of variance and a post hoc Tukey's test were performed to compare bond strength values at a significance level of 0.05. Statistical analysis was performed using a statistical software package (Minitab, Minitab Inc.; State College, PA, USA).
| Results|| |
All the microtensile bond strength (μTBS) data are presented in [Table 2]. Statistically significant cross-interaction among the three main factors was found (P = 0.029).
|Table 2: Bond strength mean in MPa (standard deviation) (tested sps/premature failures) to each experimental group|
Click here to view
In general, all adhesive systems assessed used in ER strategy produced higher values in sound dentin compared to artificially CAD. For SE strategy, the μTBS values were similar between sound and artificially CAD, except those obtained with SU, which were higher in sound dentin.
All multi-mode systems presented similar μTBS values, regardless of the etching strategy in each substrate condition. The same was not valid for adhesive systems considered as controls, as SB showed higher values than CS in sound dentin.
Adhesive/mixed failure pattern was predominant for all experimental groups [Figure 1]. Cohesive failures (resin or dentin) seemed to be more frequent in sound dentin.
|Figure 1: Fracture type distribution per experimental groups and substrates (sound– SND and caries affected dentin-DEM)|
Click here to view
| Discussion|| |
According to the obtained results, the versatility concept of multi-mode adhesives that allows the clinicians to choose either etch-and-rinse or a self-etch protocol seems to be accurate, considering each dentin condition separately. Nonetheless, bond strength values for all adhesive systems tested in the etch-and-rinse strategy were significantly higher in sound dentin when compared to artificially induced CAD. These findings indicate different interaction patterns in each substrate since sound and demineralized dentin present differences in structural characteristics. CAD is more porous than sound dentin due to the mineral loss in the demineralization process. The thicker hybrid layer has been found in demineralized dentin, which suggests that the increase in porosity allows a great diffusion of primers and monomers.
For MMAS, the etching strategy did not affect bond strength values considering each substrate condition separately. Other studies have also found no differences on immediate bonding of universal adhesive systems using etch-and-rinse and self-etch protocols in sound dentin.,, Similarly, the etching strategy did not influence on bond strength to artificially induced CAD, as observed previously in artificially induced CAD in the primary , and permanent teeth.
The study findings are partially in accordance with previous studies ,, that found the improved bond strength of adhesive systems to sound dentin. Higher bond strength values were found to sound dentin when compared to artificially induced CAD, only when MMAS were used in etch-and-rinse mode. The aggressiveness of etch-and-rinse strategy in an artificially induced CAD may produce a thicker layer of demineralization  and probably incomplete infiltration by resin components.
Multi-mode adhesives used in the self-etch mode were not influenced by substrate condition since almost all systems presented similar bond strength values. Only the SU produced higher bond strength values in SE strategy in sound dentin compared to artificially induced CAD. CS, AB and PB (both in SE strategy) presented similar bond strength on both substrates. The performance of these adhesives in both substrates assent with other studies,, that showed no differences on sound and artificially CAD for self-etch adhesives. Moreover, the less acidity of self-etch adhesives when applied on CAD may reduce the depth difference between conditioned area and monomer infiltration.
The composition of multi-mode adhesives may play an important role in bond strength values. A recent systematic review revealed that acidic monomers of multi-mode adhesives might have an influence on bond strength values. Rosa et al., found that ER strategy enhances the performance of ultra-mild adhesives. A reasonable explanation for that behavior is that ultra-mild adhesives in SE approach could not be able to properly conditioning and preparing the dentin substrate. However, there were no significant differences between strategies, supporting the main purpose of MMAS: Versatility to be used in both strategies without compromising the performance, at least in immediate evaluation.
Considering the adhesives used as controls, SB performed better than CS on the sound dentin. Other studies , already showed such behavior for both adhesive systems on the sound substrate. A possible explanation for the decrease the performance of self-etch gold standard is the fact that this was the only adhesive tested which manufacturer does not recommend the active application. Studies , revealed that active application enhances immediate and long-term bond strength of self-etch adhesives. The fact that CS is available on the market for a long time could explain manufacturer's instruction without active application. However, this issue does not impair the clinical performance of CS, as the clinical effectiveness of CS on noncarious cervical lesions remained excellent even after 13 years of follow-up.
The lower mineral content of artificially induced CAD makes them similar to natural CAD, a clinically relevant substrate. Several studies using a similar methodology to create artificially CAD found that this substrate present demineralization on intertubular dentin and an opening of dentinal tubules. These findings support the use of the pH-cycling method to induce artificially CAD for testing the adhesive interfaces. In addition, a study  that investigated an artificially CAD model for in vitro bonding studies reported that the μTBS values to CAD were lower than those obtained for sound dentin, but were not influenced by the type of caries. These findings support the use of pH cycling as a suitable methodology to induce artificially CAD avoiding the great variability of natural caries.
Although the pH-cycling model for artificial caries induction is supported on the literature, we should consider that, for in vitro studies, it is not possible to simulate all the physiological changes that occur in a clinical situation, such as the response of dentin-pulp complex like dentin sclerosis and tertiary dentin formation. It is likely that these pulp defense responses cause micromorphological changes in dentin, and their effect on adhesion establishment cannot be completely assessed in an in vitro study design.
Bovine teeth are considered a viable substrate for adhesive in vitro investigations. A recent systematic review with meta-analysis  supported the use of bovine teeth on bond strength studies of adhesive systems. Thereby, the use of bovine teeth for in vitro studies as an alternative to human teeth seems advantageous, since bovine teeth are obtained easily and aplenty, unlike human teeth.
Considering obtained results, we accepted the first null hypothesis, since adhesive systems showed similar performance for both strategies on each substrate condition individually. The second null hypothesis was rejected since the bond strength of the MMAS were influenced by substrate condition when applied in etch-and-rinse mode. Long-term studies are necessary and already are being developed by our study group to investigate the bond strength behavior of these multi-mode adhesives on different substrate condition.
| Conclusion|| |
The etching strategy does not influence the bond strength of multi-mode adhesives to sound or artificially CAD, considering each substrate separately. The dentin condition has a great influence on the immediate performance of multi-mode adhesives applied in etch-and-rinse mode– artificially induced CAD presented lower values than sound dentin.
We would like to thank the CAPES for the financial support and scholarship.
Financial support and sponsorship
Conflicts of interest
There are no conflicts of interest.
| References|| |
Hanabusa M, Mine A, Kuboki T, Momoi Y, Van Ende A, Van Meerbeek B, et al.
Bonding effectiveness of a new 'multi-mode' adhesive to enamel and dentine. J Dent 2012;40:475-84.
Marchesi G, Frassetto A, Mazzoni A, Apolonio F, Diolosà M, Cadenaro M, et al.
Adhesive performance of a multi-mode adhesive system: 1-year in vitro
study. J Dent 2014;42:603-12.
Chen C, Niu LN, Xie H, Zhang ZY, Zhou LQ, Jiao K, et al.
Bonding of universal adhesives to dentine – Old wine in new bottles? J Dent 2015;43:525-36.
Luque-Martinez IV, Perdigão J, Muñoz MA, Sezinando A, Reis A, Loguercio AD, et al.
Effects of solvent evaporation time on immediate adhesive properties of universal adhesives to dentin. Dent Mater 2014;30:1126-35.
Muñoz MA, Luque-Martinez I, Malaquias P, Hass V, Reis A, Campanha NH, et al
. In vitro
longevity of bonding properties of universal adhesives to dentin. Oper Dent 2015;40:282-92.
Wagner A, Wendler M, Petschelt A, Belli R, Lohbauer U. Bonding performance of universal adhesives in different etching modes. J Dent 2014;42:800-7.
Rosa WL, Piva E, Silva AF. Bond strength of universal adhesives: A systematic review and meta-analysis. J Dent 2015;43:765-76.
Schwendicke F, Dörfer CE, Paris S. Incomplete caries removal: A systematic review and meta-analysis. J Dent Res 2013;92:306-14.
Yoshiyama M, Tay FR, Doi J, Nishitani Y, Yamada T, Itou K, et al.
Bonding of self-etch and total-etch adhesives to carious dentin. J Dent Res 2002;81:556-60.
Nakajima M, Sano H, Burrow MF, Tagami J, Yoshiyama M, Ebisu S, et al.
Tensile bond strength and SEM evaluation of caries-affected dentin using dentin adhesives. J Dent Res 1995;74:1679-88.
Scholtanus JD, Purwanta K, Dogan N, Kleverlaan CJ, Feilzer AJ. Microtensile bond strength of three simplified adhesive systems to caries-affected dentin. J Adhes Dent 2010;12:273-8.
Nicoloso GF, Antoniazzi BF, Lenzi TL, Soares FZ, Rocha RO. Is there a best protocol to optimize bond strength of a universal adhesive to artificially induced caries-affected primary or permanent dentin? J Adhes Dent 2016;18:441-6.
Van Meerbeek B, De Munck J, Mattar D, Van Landuyt K, Lambrechts P. Microtensile bond strengths of an etch& rinse and self-etch adhesive to enamel and dentin as a function of surface treatment. Oper Dent 2003;28:647-60.
Lenzi TL, Soares FZ, Raggio DP, Pereira GK, Rocha RO. Dry-bonding etch-and-rinse strategy improves bond longevity of a universal adhesive to sound and artificially-induced caries-affected primary dentin. J Adhes Dent 2016;18:475-82.
Lenzi TL, Raggio DP, Soares FZ, Rocha Rde O. Bonding performance of a multimode adhesive to artificially-induced caries-affected primary dentin. J Adhes Dent 2015;17:125-31.
Erhardt MC, Rodrigues JA, Valentino TA, Ritter AV, Pimenta LA.In vitro
microTBS of one-bottle adhesive systems: Sound versus artificially-created caries-affected dentin. J Biomed Mater Res B Appl Biomater 2008;86:181-7.
Aguilar-Mendoza JA, Rosales-Leal JI, Rodríguez-Valverde MA, González-López S, Cabrerizo-Vílchez MA. Wettability and bonding of self-etching dental adhesives. Influence of the smear layer. Dent Mater 2008;24:994-1000.
Hebling J, Castro FL, Costa CA. Adhesive performance of dentin bonding agents applied in vivo
and in vitro
. Effect of intrapulpal pressure and dentin depth. J Biomed Mater Res B Appl Biomater 2007;83:295-303.
Loguercio AD, Stanislawczuk R, Mena-Serrano A, Reis A. Effect of 3-year water storage on the performance of one-step self-etch adhesives applied actively on dentine. J Dent 2011;39:578-87.
Pleffken PR, de Almeida Lourenço AP, Torres CR, Bühler Borges A. Influence of application methods of self-etching adhesive systems on adhesive bond strength to dentin. J Adhes Dent 2011;13:517-25.
Peumans M, De Munck J, Van Landuyt K, Van Meerbeek B. Thirteen-year randomized controlled clinical trial of a two-step self-etch adhesive in non-carious cervical lesions. Dent Mater 2015;31:308-14.
Marquezan M, Osorio R, Ciamponi AL, Toledano M. Resistance to degradation of bonded restorations to simulated caries-affected primary dentin. Am J Dent 2010;23:47-52.
Lenzi TL, Tedesco TK, Calvo AF, Ricci HA, Hebling J, Raggio DP, et al.
Does the method of caries induction influence the bond strength to dentin of primary teeth? J Adhes Dent 2014;16:333-8.
Joves GJ, Inoue G, Nakashima S, Sadr A, Nikaido T, Tagami J, et al.
Mineral density, morphology and bond strength of natural versus artificial caries-affected dentin. Dent Mater J 2013;32:138-43.
Soares FZ, Follak A, da Rosa LS, Montagner AF, Lenzi TL, Rocha RO, et al.
Bovine tooth is a substitute for human tooth on bond strength studies: A systematic review and meta-analysis of in vitro
studies. Dent Mater 2016;32:1385-93.
Dr. Fabio Zovico Maxnuck Soares
Rua Floriano Peixoto, 1184, Santa Maria, RS, 97015-270
Source of Support: None, Conflict of Interest: None
[Table 1], [Table 2]
| Article Access Statistics|
| Viewed||418 |
| Printed||12 |
| Emailed||0 |
| PDF Downloaded||56 |
| Comments ||[Add] |